Crystal structures of (barium, europium) platinum trigermanium, Ba~1- x~EuxPtGe3 (x = 0, 0.27, 1)
Demchyna, R.; Prots, Yu.; Schnelle, W.; Burkhardt, U.; Schwarz, U.; Zeitschrift für Kristallographie - New Crystal Structures 221 (2006) 109–111; doi:

data_8102937
_publ_section_title
;
Crystal structures of (barium, europium) platinum trigermanium, Ba~1-
x~EuxPtGe3 (x = 0, 0.27, 1)
;
_journal_issue                   2
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              109
_journal_page_last               111
_journal_volume                  221
_journal_year                    2006
_chemical_formula_sum            'Eu Ge3 Pt'
_chemical_formula_weight         564.82
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2006-02-02T10:02:43-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.4633(1)
_cell_length_b                   4.4633(1)
_cell_length_c                   10.0625(4)
_cell_measurement_temperature    293(2)
_cell_volume                     200.456(10)
_computing_cell_refinement       'CSD (Akselrud, 1993)'
_computing_data_collection       'CrystalClear (Rigaku Corp., 2000)'
_computing_data_reduction        'CrystalClear (Rigaku Corp., 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295.15
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measurement_device       'Rigaku AFC7'
_diffrn_measurement_method       oscillation
_diffrn_radiation_detector       'Mercury CCD'
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_source         'Sealed Tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.030
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            843
_diffrn_reflns_reduction_process 'Lp corrections applied'
_diffrn_reflns_theta_max         32.99
_diffrn_reflns_theta_min         4.05
_diffrn_source_current           48.0000
_diffrn_source_power             2.4000
_diffrn_source_voltage           50.0000
_exptl_absorpt_coefficient_mu    72.176
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5201
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            metalic
_exptl_crystal_density_diffrn    9.358
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular shape'
_exptl_crystal_F_000             474
_exptl_crystal_size_max          0.040
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.015
_refine_diff_density_max         1.228
_refine_diff_density_min         -2.434
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.026(14)
_refine_ls_extinction_coef       0.0168(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_matrix_type           full
_refine_ls_number_parameters     14
_refine_ls_number_reflns         241
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_gt           0.018
_refine_ls_shift/su_max          0.092
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.035
_reflns_number_gt                241
_reflns_number_total             241
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            409869.cff
_cod_data_source_block           EuGe3Pt
_cod_depositor_comments
;
The following automatic conversions were performed:
'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 
;
_cod_original_cell_volume        200.46(1)
_cod_database_code               8102937